The production of concentrated dispersions of few-layer graphene by the direct exfoliation of graphite in organosilanes
© Nuvoli et al.; licensee Springer. 2012
Received: 1 October 2012
Accepted: 12 November 2012
Published: 13 December 2012
We report the formation and characterization of graphene dispersions in two organosilanes, 3-glycidoxypropyl trimethoxysilane (GPTMS) and phenyl triethoxysilane (PhTES) as new reactive solvents. The preparation method was mild and easy and does not produce any chemical modification. The dispersions, which exhibit the Tyndall effect, were characterized by TEM and Raman spectroscopy to confirm the presence of few-layer graphene. Concentrations as high as 0.66 and 8.00 mg/ml were found for PhTES and GPTMS, respectively. The latter is one of the highest values reported for a dispersion of graphene obtained by any method. This finding paves the way for the direct synthesis of polymer nanofiller-containing composites consisting of graphene and reactive silanes to be used in sol–gel synthesis, without any need for solvent removal, thus preventing graphene reaggregation to form graphite flakes.
KeywordsGraphene Organosilanes High concentration Liquid exfoliation
Graphene, with its unique physical properties[1–4], is one of the most exciting nanomaterials discovered in the last years. A particularly promising graphene production technique is based on the obtainment of colloidal suspensions from graphite, or its derivatives. In spite of other methods like epitaxial growth, chemical vapor deposition, and micromechanical exfoliation, this approach is both scalable, affording the possibility of high-volume production, and versatile in terms of chemical functionalization, which, on the other hand, is sometimes exploited to favor graphene obtainment and its dispersion. Colloidal graphene suspensions may be advantageous in that they could be used for a wide range of applications including: spray coating, vacuum filtration, or drop casting; moreover, by mixing them with polymers, graphene-based polymer composites can be prepared. In these production methods, the key challenge involves the exfoliation of graphitic materials in a liquid that can disperse graphene sheets in a stable way.
One of the most common methods to obtain graphene by this technique involves the dispersion and exfoliation of graphene oxide. This material consists of graphene sheets which are chemically functionalized with groups such as hydroxy and epoxide, which stabilize them in water. However, this functionalization results in considerable damaging of graphene electronic structure, which becomes a semiconductor. While the epoxide functionalities can be removed by reduction, the hydroxy and carboxy cannot be removed. Recently, a significant breakthrough was made when some research groups showed that graphite could be exfoliated by non-chemical solution phase methods with solvents[11–13] or surfactants[14, 15]. The energy required to exfoliate graphene is balanced by the solvent-graphene interaction for compounds whose surface energy matches that of graphene. By this technique, our research group obtained few-layer graphene sheets by sonication of graphite with N-methyl pyrrolidone, isocyanates, N-vinyl caprolactam, a commercial ionic liquid, and an acrylate, thus, achieving a graphene concentration as high as 2.21, 3.78, 5.00, 5.33 and 9.45 mg/ml, respectively, which are among the highest reported so far in any liquid.
Analogously in the present work, we used reactive organosilane compounds to obtain stable graphene dispersions. Organosilanes are characterized by the basic structure R n Si(OR)4 − n, where R is an alkyl, aryl, or organofunctional group, and OR is generally a methoxy or ethoxy group, which can react with the hydroxyl groups and liberate methanol or ethanol. Organo(alkoxy)silanes are used in coating applications for surface treatment, as additives in paints, inks, and adhesives, and as reactive intermediates for silicone resin syntheses and organic resin modifications: The alkoxy group can be exploited for the linkage with inorganic substrates, pigments, fillers and hydroxy functionalized polymers. Organo(alkoxy)silanes are used as precursors for the synthesis of inorganic–organic hybrid materials. In particular, 3-glycidoxypropyl trimethoxysilane (GPTMS) and phenyl triethoxysilane (PhTES) are two of the most commonly used for these purposes. Hydrolysis of the methoxy or ethoxy groups of GPTMS and PhTES gives rise to silanol groups which can condense to form silicate networks. Moreover, GPTMS has an epoxy ring that can be used for organic network formation, for instance, through condensation with diethylenetriamine or ethylenediamine at room temperature; this dual functionality makes GPTMS a strategic component for the preparation of polymer hybrids.
In the present work, for the first time PhTES and GPTMS were used for dispersing graphene by direct graphite sonication, without any chemical manipulation. The resulting material was thoroughly characterized by using Raman and UV spectroscopies. Moreover, transmission electron microscopy was used for the statistical analysis concerning the distribution among mono and few-layer graphenes.
Phenyl triethoxysilane, 3-glycidoxypropyl trimethoxysilane and graphite flakes (+100 mesh) were purchased from Sigma Aldrich (Sigma-Aldrich Corporation, St. Louis, MO, USA) and used as received without further purification.
Mixtures containing various amounts of graphite flakes and organosilane (5.00 g) were put in a tubular plastic reactor (i.d. 15 mm) and placed in an ultrasonic bath (0.55 KW, water temperature ≈ 25°C) for 24 h. Then, after they were centrifuged for 30 min at 4,000 rpm, the gray to black liquid phase containing graphene was recovered.
Graphene dispersion concentration
In order to determine the graphene concentration, the above dispersion was divided into two fractions with a known volume. The first one was filtered through polyvinylidene fluoride filters (PVDF, pore size of 0.22 μm) in order to directly weigh the amount of dispersed graphene and determine the actual graphene concentration.
Determination of absorption coefficient α
The second aliquot of the above dispersion was analyzed by UV analysis with a Hitachi U-2010 spectrometer (1 cm cuvette, Hitachi Corporation, Tokyo, Japan). The above gravimetric data allowed us to determine the absorption coefficient α: from a known volume of initial dispersion, several dilutions were done and the absorbance at a wavelength of 660 nm was measured[11, 17, 24]. Absorbance versus concentration plots gave the absorption coefficient α (see Results and discussion) value.
TEM measurements were performed on a JEOL JEM-2100 TEM instrument (JEOL Ltd., Akishima, Tokyo, Japan), with a LaB6 filament, with an operating voltage of 200 kV.
For the TEM analysis, the solutions were sonicated for 5 min and then cast directly on the 200 mesh cooper grid; eventually, the solvent was evaporated at ambient conditions for 24 h.
Analyses were performed on graphene flakes obtained after vacuum filtration of dispersions on PVDF filters (pore size 0.22 μm), with a Bruker Senterra Raman microscope (Bruker Corporation, Billerica, MA, USA), using an excitation wavelength of 532 nm at 5 mW. The spectra were acquired by averaging five acquisitions of 5 s with a ×50 objective.
Results and discussion
The feasibility of using organosilanes as effective liquid dispersing media for graphene was investigated. In particular, PhTES and GPTMS were tested with the aim of preparing graphene dispersions that could be directly utilized for further uses without recovering graphene in the solid state, thus avoiding any possible restacking of it to pristine graphite and compromising any previous successful exfoliation process.
The flakes present good exfoliation degree with an average number of layers of 2.7 for GPTMS and 2.4 for PhTES; standard deviation was about 0.4 and 0.5, respectively. In both cases, only 14% of the flakes were present more than three layers. Moreover, no more than five layers have been counted in very few flakes thus indicating a narrow dispersion. These results confirm that the exfoliation process was very effective.
The disorder-related D peak is present also in the initial graphite powder, but its intensity is higher for graphene. This finding was already reported in which graphene was produced by sonication of graphite and can be attributed to the new edges produced during the sonication process: Ultrasonic treatment causes the decrease in size of the flakes compared to the original graphite, with a consequent increase of the total edge length[12, 24, 31]. Comparing the intensity of the peaks and the D/G ratio found in the case of graphene obtained in GPTMS and PhTES, only little differences can be found, thus indicating that the disorder induced by the exfoliation process is very similar. Namely, the D/G ratio is 0.47 for graphene dispersed in GPTMS and 0.65 for that dispersed in PhTES, while the reference value for graphite powder is 0.14.
On the basis of the above concentration results, some considerations about the use of the Hildebrand solubility parameters δ should be done. Indeed, Hernandez et al. stated that these parameters could be the key for envisaging the best graphene solvent media. In particular, they calculated a δ value for graphene equal to ca. 23 MPa1/2, this value being the same of N-methyl-2-pyrrolidone. However, GPTMS, the best solvent medium reported here, is characterized by δ = 14.5 MPa1/2. This value suggests that graphene solubility parameters should be revised and/or that they are not adequate for any reliable solubility prediction on this respect.
A significant improvement of the methods used so far for graphene obtainment has been carried out. Namely, the two new liquid media in which graphene was found to effectively disperse were investigated. In particular, GPTMS and PhTES were chosen as representatives of the larger family of organosilanes. Both of them are commonly used in sol–gel synthesis; moreover, GPTMS can be also used for the preparation of polymer hybrids. In detail, this compound resulted to be one of the most effective medium found so far for dispersing graphene, allowing for a concentration of this material equal to 8.00 mg/ml.
The concentration value found for PhTES is much lower (0.66 mg/ml) but, if especially compared with that of most the reported data[11, 22, 26, 27], it can be considered of interest; for instance, for the preparation of polymer composites, in which an even lower concentration of graphene might result in peculiar final properties of the resulting material[16, 18, 33–35].
The authors thank GEMPPO at the IEM-CSIC for the use of the TEM.
- Lee C, Wei X, Kysar JW, Hone J: Measurement of the elastic properties and intrinsic strength of monolayer graphene. Science 2008, 321: 385–388. 10.1126/science.1157996View Article
- Balandin AA, Ghosh S, Bao W, Calizo I, Teweldebrhan D, Miao F, Lau CN: Superior thermal conductivity of single-layer graphene. Nano Lett 2008, 8: 902–907. 10.1021/nl0731872View Article
- Bolotin KI, Sikes KJ, Jiang Z, Klima M, Fudenberg G, Hone J, Kim P, Stormer HL: Ultrahigh electron mobility in suspended graphene. Solid State Commun 2008, 146: 351–355. 10.1016/j.ssc.2008.02.024View Article
- Stoller MD, Park S, Zhu Y, An J, Ruoff RS: Graphene-based ultracapacitors. Nano Lett 2008, 8: 3498–3502. 10.1021/nl802558yView Article
- Park S, Ruoff RS: Chemical methods for the production of graphenes. Nat Nanotechnol 2009, 4: 217–224. 10.1038/nnano.2009.58View Article
- Berger C, Song Z, Li X, Wu X, Brown N, Naud C, Mayou D, Li T, Hass J, Marchenkov AN, Conrad EH, First PN, de Heer WA: Electronic confinement and coherence in patterned epitaxial graphene. Science 2006, 312: 1191–1196. 10.1126/science.1125925View Article
- Eizenberg M, Blakely JM: Carbon monolayer phase. condensation on Ni(111). Surf Sci 1970, 82: 228–236.View Article
- Novoselov KS, Geim AK, Morozov SV, Jiang D, Zhang Y, Dubonos SV, Grigorieva IV, Firsov AA: Electric field effect in atomically thin carbon films. Science 2004, 306: 666–669. 10.1126/science.1102896View Article
- Stankovich S, Dikin DA, Dommett GHB, Kohlhaas KM, Zimney EJ, Stach EA, Piner RD, Nguyen ST, Ruoff RS: Graphene-based composite materials. Nature 2006, 442: 282–286. 10.1038/nature04969View Article
- Coleman JN: Liquid exfoliation of defect-free graphene. Acc Chem Res 2012. 10.1021/ar300009f
- Hernandez Y, Nicolosi V, Lotya M, Blighe FM, Sun ZY, De S, McGovern IT, Holland B, Byrne M, Gun’Ko YK, Boland JK, Niraj P, Duesberg G, Krishnamurthy S, Goodhue R, Hutchison J, Scardaci V, Ferrari AC, Coleman JN: High-yield production of graphene by liquid-phase exfoliation of graphite. Nat Nanotechnol 2008, 3: 563–568.View Article
- Khan U, O’Neill A, Lotya M, De S, Coleman JN: High-concentration solvent exfoliation of graphene. Small 2010, 6: 864–871. 10.1002/smll.200902066View Article
- Hernandez Y, Lotya M, Shane DR, Bergin D, Coleman JN: Measurement of multicomponent solubility parameters for graphene facilitates solvent discovery. Langmuir 2010, 26: 3208–3213. 10.1021/la903188aView Article
- Lotya M, Hernandez Y, King PJ, Smith RJ, Nicolosi V, Karlsson LS, Fiona Blighe FM, De S, Wang Z, McGovern IT, Duesberg GS, Coleman JN: Liquid phase production of graphene by exfoliation of graphite in surfactant/water solutions. J Am Chem Soc 2009, 131: 3611–3620. 10.1021/ja807449uView Article
- Green AA, Hersam MC: Solution phase production of graphene with controlled thickness via density differentiation. Nano Lett 2009, 9: 4031–4036. 10.1021/nl902200bView Article
- Alzari V, Nuvoli D, Scognamillo S, Piccinini M, Gioffredi E, Malucelli G, Marceddu S, Sechi M, Sanna V, Mariani A: Graphene-containing thermoresponsive nanocomposite hydrogels of poly( N -isopropylacrylamide) prepared by frontal polymerization. J Mater Chem 2011, 21: 8727–8733. 10.1039/c1jm11076dView Article
- Sanna R, Sanna D, Alzari V, Nuvoli D, Scognamillo S, Piccinini M, Lazzari M, Gioffredi E, Malucelli G, Mariani A: Synthesis and characterization of graphene-containing thermoresponsive nanocomposite hydrogels of poly( N -vinylcaprolactam) prepared by frontal polymerization. J Polym Sci Part A: Polym Chem 2012, 50: 4110–4118. 10.1002/pola.26215View Article
- Scognamillo S, Gioffredi E, Piccinini M, Lazzari M, Alzari V, Nuvoli D, Sanna R, Piga D, Malucelli G, Mariani A: Synthesis and characterization of nanocomposites of thermoplastic polyurethane with both graphene and graphene nanoribbon fillers. Polymer 2012, 53: 4019–4024. 10.1016/j.polymer.2012.07.020View Article
- Nuvoli D, Valentini L, Alzari V, Scognamillo S, Bittolo Bon S, Piccinini M, Illescas J, Mariani A: High concentration few layer graphene sheets obtained by liquid phase exfoliation of graphite in ionic liquid. J Mater Chem 2011, 21: 3428–3431. 10.1039/c0jm02461aView Article
- Alzari V, Nuvoli D, Sanna R, Scognamillo S, Piccinini M, Kenny JM, Malucelli G, Mariani A: In situ production of high filler content graphene-based polymer nanocomposites by reactive processing. J Mater Chem 2011, 21: 3428–3431. 10.1039/c0jm02461aView Article
- Schottner G: Hybrid sol–gel-derived polymers: applications of multifunctional materials. Chem Mater 2001, 13: 3422–3435. 10.1021/cm011060mView Article
- Davis SR, Brough AR, Atkinson A: Formation of silica/epoxy hybrid network polymers. J Non-Cryst Solids 2003, 315: 197–205. 10.1016/S0022-3093(02)01431-XView Article
- Scognamillo S, Alzari V, Nuvoli D, Mariani A: Hybrid organic inorganic epoxy resins prepared by frontal polymerization. J Polym Sci Part A: Polym Chem 2010, 48: 4721–4725. 10.1002/pola.24263View Article
- Lotya M, King PJ, Khan U, De S, Coleman JN: High-concentration, surfactant-stabilized graphene dispersions. ACS Nano 2010, 4: 3155–3162. 10.1021/nn1005304View Article
- Li D, Müller MB, Gilje S, Kaner RB, Wallace GG: Processable aqueous dispersions of graphene nanosheets. Nat Nanotechnol 2008, 3: 101–105. 10.1038/nnano.2007.451View Article
- Yang Q, Pan X, Huang F, Li K: Fabrication of high-concentration and stable aqueous suspensions of graphene nanosheets by noncovalent functionalization with lignin and cellulose derivatives. J Phys Chem C 2010, 114: 3811–3816.View Article
- Khan U, Porwal H, O’Neill A, Nawaz K, May P, Coleman JN: Solvent-exfoliated graphene at extremely high concentration. Langmuir 2011, 27: 9077–9082. 10.1021/la201797hView Article
- Ferrari AC: Raman spectroscopy of graphene and graphite: disorder, electron–phonon coupling, doping and nonadiabatic effects. Solid State Commun 2007, 143: 47–57. 10.1016/j.ssc.2007.03.052View Article
- Nemanich RJ, Solin S: First- and second-order Raman scattering from finite-size crystals of graphite. Phys Rev B 1979, 20: 392–401. 10.1103/PhysRevB.20.392View Article
- Ferrari AC, Meyer JC, Scardaci V, Casiraghi C, Lazzeri M, Mauri FS, Piscanec FS, Jiang D, Novoselov KS, Roth S, Geim AK: Raman spectrum of graphene and graphene layers. Phys Rev Lett 2006, 97: 187401–187404.View Article
- Casiraghi C, Hartschuh A, Qian H, Piscanec S, Georgi C, Fasoli A, Novoselov KS, Basko DM, Ferrari AC: Raman spectroscopy of graphene edges. Nano Lett 2009, 9: 1433–1441. 10.1021/nl8032697View Article
- Suzuki N, Ishida H: Effect of the miscibility between a silane and a sizing agent on silanol condensation. J Appl Polym Sci 2003, 87: 589–598. 10.1002/app.11297View Article
- Ramanathan T, Abdala AA, Stankovich S, Dikin DA, Herrera-Alonso M, Piner RD, Adamson DH, Schniepp HC, Chen X, Ruoff RS, Nguyen ST, Aksay IA, Prud’Homme RK, Brinson LC: Functionalized graphene sheets for polymer nanocomposites. Nat Nanotechnol 2008, 3: 327–331. 10.1038/nnano.2008.96View Article
- Rafiee MA, Rafiee J, Wang Z, Song H, Yu ZZ, Koratkar N: Enhanced mechanical properties of nanocomposites at low graphene content. ACS Nano 2009, 3: 3884–3890. 10.1021/nn9010472View Article
- Verdejo R, Barroso-Bujans F, Rodriguez-Perez MA, de Saja JA, Lopez-Manchado MA: Functionalized graphene sheet filled silicone foam nanocomposites. J Mater Chem 2008, 18: 2221–2226. 10.1039/b718289aView Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.